- Nano Express
- Open Access

# A general formalism for the determination of the effective mass of the nanoscale structural inhomogeneities of the domain wall in uniaxial ferromagnets

- Andriy Shevchenko
^{1}Email author and - Maksym Barabash
^{2}

**10**:159

https://doi.org/10.1186/s11671-015-0861-z

© Shevchenko and Barabash; licensee Springer. 2015

**Received:**14 October 2014**Accepted:**14 March 2015**Published:**2 April 2015

## Abstract

On the basis of the method of gyrotropic Thiele forces, we build a formalism that allows the determination of the effective mass of the nanoscales structural elements of the domain wall (DW): vertical Bloch line and Bloch point in uniaxial ferromagnets. As shown, the effective mass of these magnetic inhomogeneities depends on the value of the gyrotropic domain wall bend that is created by their movement.

## PACS

- 61.46. − w
- 03.65. − w
- 03.65.Db

## Keywords

- Gyrotropic Thiele force
- Uniaxial ferromagnet
- The domain wall
- The vertical Bloch line
- The Bloch point
- Gyrotropic bend
- The effective mass

## Background

The study of structural localized inhomogeneities of the domain walls (DWs) of domain-containing magnetic materials is one of the topical problems in the solid state physics. Of special interest are the distributions of the magnetization vector \( \overrightarrow{M} \) in the DWs of uniaxial ferromagnets: the vertical Bloch lines (BLs) and Bloch points (BPs) (see [1] and review [2]). The vertical BL and BP are stable nanoscale formations (approximately 10^{2} nm), which significantly affect the dynamics of the DW in external magnetic fields. Furthermore, BLs and BPs are considered as promising carriers of information in high performance memory devices with a superdense magnetic memory [3].

Many aspects related to the generation, stability, and dynamics of the vertical BL and BP have been studied. At the same time, some provisions that characterize the given inhomogeneities require more detailed consideration. One of these problems is to determine *m*
_{
L,BP
} - the effective masses of the vertical BL and BP. The effective mass is an important dynamical characteristic caused by the quasiparticle approach to the investigation of vertical BL and BP movement. Accordingly, *m*
_{
L,BP
} are determined from the ‘kinetic potentials’ constructed on the basis of systems of integrodifferential equation solutions of the BL and BP dynamics. This approach presents significant difficulties [4-7], and it would be laudable to build a simpler theoretical formalism for finding *m*
_{
L,BP
} in the DW of different domain configurations. Another difficulty with the previous formalism is related to the dependence of the BL and BP parameters of the quantum effects, which take place for these magnetic structures in the subhelium temperature range, on their effective mass expressions [8,9]. This aspect is especially important for spintronics materials such as cylindrical nanowires and nanostripes in which is the presence of structures similar to BLs and BPs [10-13]. The construction of a general method, which allows the determination of the effective mass of nanoscale structural inhomogeneities of the DW in ferromagnets with strong uniaxial anisotropy, using the concept of a gyrotropic (gyroscopic) Thiele force acting on a moving magnetization distribution [14] is the aim of our work.

## Methods

### Problem solving and discussion

*θ*and

*φ*, respectively. The functional dependences of these angles corresponding to the static states of the DW and BL are well known and have the form [1]

**Δ**is the DW width, \( \Lambda =\Delta \sqrt{Q} \) is the BL characteristic size, and

*Q*is the material quality factor (the ratio of the magnetic anisotropy energy to the magnetostatic one),

*Q*> > 1.

*M*

_{ S }is the saturation magnetization,

*γ*is the gyromagnetic ratio, \( \overrightarrow{\mathrm{g}}=- \sin \theta \left[\overrightarrow{\nabla}\theta \times \overrightarrow{\nabla}\phi \right] \) is the gyrotropic vector, and \( \overrightarrow{v}=\left({v}_x{\overrightarrow{e}}_x,\;{v}_y{\overrightarrow{e}}_y\right) \) is the velocity of the magnetic inhomogeneity.

*x*and

*y*(in given case) and characterizes the link between its parts - BL and DW. This allows us to consider the \( {\overrightarrow{\mathrm{f}}}_{\mathrm{g},x,y} \) components as interaction forces. So, the \( {\overrightarrow{\mathrm{f}}}_{\mathrm{g},x} \) component manifests as a force that acts from the moving domain wall on the vertical BL. In turn, the component of \( {\overrightarrow{\mathrm{f}}}_{\mathrm{g},y} \) acting on the DW is caused by the dynamics of the BL. The result is a deformation of the DW, namely a gyrotropic bend that can be characterized in terms of the Slonczewski approach [1] by the coordinate of the normal displacement of its center -

*q*(

*ξ*), where

*ξ*=

*x*−

*v*

_{ L }

*t*, and

*v*

_{ L }is the BL velocity. In this case, external to the DW force \( {\overrightarrow{\mathrm{f}}}_{\mathrm{g},y} \) produces the work with the average value \( \overline{W} \) that is related to the kinetic energy of the BL as follows

Here *q*
_{
ξ → 0} is DW displacement in the BL center. It is this equation and will be the basis for finding the effective mass of the DW structural elements. We will consider its application on specific examples.

*H*

_{ g }, the system of equations of DW dynamics has form [4]

*ψ*(

*ξ*) is angle of the vector \( \overrightarrow{M} \) in the DW center with axis OX,

*ω*

_{ M }= 4

*πγM*

_{ S }, and

*M*

_{ S }is the saturation magnetization,

*f*=

*H*

_{ g }Δ/4

*πM*

_{ S }.

*f*< <1 and

*v*

_{ L }< <Λ

*ω*

_{ M }and we obtain from (4)

*ψ*(

*ξ*) =

*φ*(

*ξ*) and using formulae (1) to (3), (5), we find the effective mass of the vertical BL

Note that expression (6) is the same as the formula for *m*
_{
L
} from article [4] lending credence to formalism presented here. In our case, we did not need the solution of the system Equation (4). We have found the asymptotic expression for the gyrotropic bend of the domain wall *q*
_{
ξ → 0}, which simplifies the study of the problem.

## Results and discussion

The dependence of the effective mass on the DW gyrotropic bend value caused by the motion of the BL indicates an inertial character of *m*
_{
L
}. In this case, a decrease in the field of stabilization of the domain wall *H*
_{
g
} should result in an increase of *q*
_{
ξ → 0} and, accordingly, *m*
_{
L
}. This agrees with formula (6): \( {m}_L\sim 1/\sqrt{f} \). In turn, from the system of equations (4), it is easy to show that *m*
_{
L
} ~ *f*
^{−1} for values *f*> > 1. The dependence of the effective mass of the vertical BL on the gradient of the bias field stabilizing DW indicates the unstable natural motion of ‘hard’ DW (DW with complex interior structure), which is also reflected in the quadratic character of the DW spectrum oscillations [15]. Obviously, an external magnetic field is necessary for stabilizing the DW in the case of vertical BL motion.

*m*

_{ DW }= (2

*πΔγ*

^{2})

^{− 1}is the DW effective mass [1]. Note that the viscosity of the system is taken into account by introducing into the balance of forces a dissipative linear vector function [16], which, to simplify the consideration of the problem, we do not consider in our article. Its effect on the stationary motion of the BL and BP results in finite values of the mobility of the DW structural inhomogeneities, causing negligibly small additions to their effective masses [1,6,7]. However, in yttrium-iron garnets, where the viscosity is due to an exchange relaxation of the magnetization vector [17], the viscosity can considerably affect the BP dynamics [18]. Therefore, in these materials it is necessary to consider some given factor in the determining of the BP effective mass.

*ẋ*

_{0}is the BL velocity,

*h*is film thickness,

*f*

_{ c }and

*k*

_{ c }are the respective critical values of the bias field gradient and wave vector characterizing DW bending instability [19], and

*K*

_{0,1}(

*x*) are the McDonald functions.

*m*

_{ L,f }- the effective mass of the vertical BL in DW of magnetic film. The result (provide a reference to the final equation) coincides with the corresponding formula given in article [6]

*β*

_{ L }is the angle coordinate of the BL center,

*a*= 2

*r*/

*h*,

*r*is the domain radius,

*l*is the characteristic length, and

*S*

_{ n }(

*a*) is the Thiele functions [20]. Then using Equation (3), we find that

*m*

_{ L,BD }- the effective mass of the vertical BL in the DW of magnetic bubble - can be written as

The identity of the given formula to similar expression from article [7] again demonstrates the universality of our formalism in a variety of domain systems.

*R*< Λ, where \( R=\sqrt{x^2+{z}^2} \). It is the area that mainly contributes to the effective mass of the Bloch point -

*m*

_{ BP }. In this region, there is a ‘vortex-like’ deformation of the BL magnetic structure, which is described by the system of equations [5]

*φ = arctgM*

_{ y }/

*M*

_{ x }.

*φ*(

*z*,

*x*) can be defined from the second equation of system (8) and has the form

*R*< Λ that corresponds to core structural deformation of the Bloch line by BP, it is clear that Equation (3) can be used to estimate

*m*

_{ BP }. For this purpose, assuming

*z*=

*z*−

*v*

_{ z }

*t*(

*v*

_{ z }is BP velocity) from formulae (1) and (2), and taking into account expression (9), we find that the force causing the DW gyrotropic bend can be expressed as

*f*< <1, and using formulae (3) and (10), we find an estimation of the BP effective mass, which coincides with the corresponding result in the article [5]:

An analysis of this expression shows that *m*
_{
BP
} does not depend on the bias field gradient, in contrast to the dependence of the effective mass on the vertical BL (see expression (6)). This results from the local character of the DW area distortion by the Bloch point (~Λ^{2}), the nature of which is determined by the surface tension of the domain wall (the terms ~ Λ^{2}∂/∂*x*
^{2} and ~ Λ^{2}∂/∂*z*
^{2} in the first equation of the system (8)). In turn, the deformation of the domain wall caused by the moving BL occurs along the entire line of the inhomogeneity, resulting in the displacement of the domain wall. Therefore, the vertical BL effective mass is determined by the bias field gradient stabilizing DW.

*f*> > 1, the singularity at the BP center can be eliminated by integrating over the BP volume. Indeed, from formula (2) and the first equation of the system (8), we define a gyroscopic force \( {\mathrm{f}}_{\mathrm{g},y}=-\frac{M_S}{\gamma } \sin \theta \frac{\partial \theta }{\partial y}\frac{\partial \varphi }{\partial z}{v}_z \) and coordinate of the DW normal displacement \( q=\Delta {\omega}_M^{-1}{f}^{-1}\frac{\partial \varphi }{\partial z}{v}_z \). Assuming the lower limit of the integral to be equal to Δ, we find and expression for work \( \overline{W}=\frac{1}{2}{\displaystyle \int {\mathrm{f}}_{\mathrm{g},y}\kern0.15em qdxdydz} \) and, using Equation (3), we arrive at an expression for the BP effective mass

The resulting expression differs only in terms of coefficients with the corresponding expression for *m*
_{
BP
} in article [5]. The effective mass of the BP in this case is determined by the external field *H*
_{
g
} and tends to zero with the DW gyrotropic bend at *f* → ∞.

These examples show that the formalism presented here, which incorporates our simple method for finding the effective masses of the vertical BL and BP, agrees well with all previously known results on this subject. Moreover, because of its generality, it can be extended to other ‘hard’ DW systems, such as dumbbell- and strip-shaped domains.

It should also be noted that expressions (2) and (3) are applicable to any moving magnetization distribution. Therefore, our formalism does not depend on the type of the ferromagnet or inhomogeneity. In this article, we have considered how local nanoscale inhomogeneities affect the interior structure of DWs in uniaxial ferromagnets classified as the vertical BL and BP.

## Conclusions

We have created a simplified formalism for finding of the effective mass of structural inhomogeneities of the DW - the vertical Bloch line and Bloch point in different domain systems of uniaxial ferromagnetic materials. It has been shown that the effective mass of the vertical BL and BP depends on the DW bend value and arises from their dynamics. At the same time, in the case of the BL, the gyrotropic bend of DW is determined by the external magnetic field stabilizing DW. In turn, the deformation of the DW due to the motion of the Bloch point is local in character and is caused both by the field stabilization of the DW and its surface tension.

## Declarations

## Authors’ Affiliations

## References

- Malozemoff AP, Slonczewski JC. Magnetic domain walls in bubble materials. New York: Academic; 1979.Google Scholar
- Volkov VV, Bokov VA. Domain wall dynamics in ferromagnets. Phys Sol State. 2008;50:199–228.View ArticleGoogle Scholar
- Konishi A. A new-ultra-density solid state memory: Bloch line memory. IEEE Trans Magn. 1983;19:1838–40.View ArticleGoogle Scholar
- Zvezdin AK, Popkov AF. Dynamics of Bloch lines in ferromagnet. JETP. 1986;64:1059–64.Google Scholar
- Kufaev YA, Sonin EB. Dynamics of a Bloch point (point soliton) in a ferromagnet. JETP. 1989;68:879.Google Scholar
- Dorman VL, Sobolev VL, Shevchenko AB. Dynamics of domain wall containing a Bloch line. JMMM. 1991;94:293.View ArticleGoogle Scholar
- Dorman VL, Sobolev VL, Shevchenko AB. Bloch lines dynamics in domain wall of magnetic bubble. JMMM. 1993;124:221.View ArticleGoogle Scholar
- Shevchenko AB. Quantum tunneling of a Bloch line in the domain wall of a cylindrical magnetic domain. Techn Phys. 2007;52:1376.View ArticleGoogle Scholar
- Shevchenko AB, Yu M, Barabash. The Bloch point in uniaxial ferromagnets as a quantum mechanical object. Nanoscale Research Lett. 2014;9:132.View ArticleGoogle Scholar
- Klaui M, Vaz CAF, Bland JAC. Head-to-head domain-wall phase diagram in mesoscopic ring magnets. Appl Phys Lett. 2004;85:5637.View ArticleGoogle Scholar
- Laufenberg M, Backes D, Buhrer W. Observation of thermally activated domain wall transformations. Appl Phys Lett. 2006;88:052507.View ArticleGoogle Scholar
- Takagi S, Tatara G. Macroscopic quantum coherence of chirality of a domain wall in ferromagnets. Phys Rev B. 1996;54:9920.View ArticleGoogle Scholar
- Vukadinovic N, Boust F. Three-dimensional micromagnetic simulations of multidomain bubble-state excitation spectrum in ferromagnetic cylindrical nanodots. Phys Rev B. 2008;78:184411.View ArticleGoogle Scholar
- Thiele AA. Steady-state motion of magnetic domains. Phys Rev Lett. 1973;30:230.View ArticleGoogle Scholar
- Thiele AA. Excitation spectrum of a magnetic domain wall containing Bloch lines. Phys Rev B. 1976;14:3130.View ArticleGoogle Scholar
- Thiele AA. Applications of the gyrocoupling vector and dissipation dyadic in the dynamics of the magnetic domains. J Appl Phys. 1974;45:375.View ArticleGoogle Scholar
- Bar’yakhtar VG. Phenomenological description of relaxation processes in magnetic materials. JETP. 1984;60:863.Google Scholar
- Galkina EG, Ivanov BA, Stephanovich VA. Phenomenological theory of Bloch point relaxation. JMMM. 1993;118:373.View ArticleGoogle Scholar
- Shlomann E. Wave propagation along domain walls in magnetic films. IEEE Trans Magn. 1974;10:11.View ArticleGoogle Scholar
- Thiele AA. Theory of static stability of cylindrical domains in uniaxial platelets. J Appl Phys. 1970;41:1139.View ArticleGoogle Scholar

## Copyright

This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.